# Assessing the Influence of Zeolite Composition on Oxygen-Bridged Diamino Dicopper(II) Complexes in Cu-CHA DeNOx Catalysts by Machine Learning-Assisted X-ray Absorption Spectroscopy

Andrea Martini, Chiara Negri, Luca Bugarin, Gabriele Deplano, Reza K. Abasabadi, Kirill A. Lomachenko, Ton V. W. Janssens, Silvia Bordiga, Gloria Berlier, Elisa Borfecchia

► To cite this version:

Andrea Martini, Chiara Negri, Luca Bugarin, Gabriele Deplano, Reza K. Abasabadi, et al. Assessing the Influence of Zeolite Composition on Oxygen-Bridged Diamino Dicopper(II) Complexes in Cu-CHA DeNOx Catalysts by Machine Learning-Assisted X-ray Absorption Spectroscopy. Journal of Physical Chemistry Letters, 2022, 13 (26), pp.6164–6170. 10.1021/acs.jpclett.2c01107. hal-05075964

HAL Id: hal-05075964

https://hal.science/hal-05075964v1

Submitted on 20 May 2025

HAL is a multi-disciplinary open access
archive for the deposit and dissemination of sci-
entific research documents, whether they are pub-
lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.

L'archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d'enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.

<figure><img src="image_1.png" /></figure>

Distributed under a Creative Commons Attribution 4.0 International License
# Assessing the Influence of Zeolite Composition on Oxygen-Bridged Diamino Dicopper(II) Complexes in Cu-CHA DeNOₓ Catalysts by Machine Learning-Assisted X-ray Absorption Spectroscopy

Andrea Martini, Chiara Negri, Luca Bugarin, Gabriele Deplano, Reza K. Abasabadi, Kirill A. Lomachenko, Ton V. W. Janssens, Silvia Bordiga, Gloria Berlier, and Elisa Borfecchia*

<figure><img src="image_2.png" /></figure>

Cite This: J. Phys. Chem. Lett. 2022, 13, 6164–6170

<figure><img src="image_3.png" /></figure>

Read Online

## ACCESS

<figure><img src="image_4.png" /></figure>

Metrics & More

<figure><img src="image_5.png" /></figure>

Article Recommendations

Supporting Information

**ABSTRACT:** Cu-exchanged chabazite is the catalyst of choice for NOₓ abatement in diesel vehicles aftertreatment systems via ammonia-assisted selective catalytic reduction (NH₃-SCR). Herein, we exploit *in situ* X-ray absorption spectroscopy powered by wavelet transform analysis and machine learning-assisted fitting to assess the impact of the zeolite composition on NH₃-mobilized Cu-complexes formed during the reduction and oxidation half-cycles in NH₃-SCR at 200 °C. Comparatively analyzing well-characterized Cu-CHA catalysts, we show that the Si/Al ratio of the zeolite host affects the structure of mobile dicopper(II) complexes formed during the oxidation of the [Cu¹(NH₃)₂]⁺ complexes by O₂. Al-rich zeolites promote a planar coordination motif with longer Cu–Cu interatomic distances, while at higher Si/Al values, a bent motif with shorter internuclear separations is also observed. This is paralleled by a more efficient oxidation at a given volumetric Cu density at lower Si/Al, beneficial for the NOₓ conversion under NH₃-SCR conditions at 200 °C.

<figure><img src="image_6.png" /></figure>

Cu-exchanged chabazite (Cu-CHA) currently is the catalyst of choice for the ammonia-assisted selective catalytic reduction (NH₃-SCR) of harmful NOₓ in diesel vehicles aftertreatment systems.¹⁻³ The NH₃-SCR technology relies on the reaction of NO and NH₃ in the presence of O₂, to form N₂ and H₂O as benign products, according to the overall stoichiometry 4NH₃ + 4NO + O₂ → 4 N₂ + 6 H₂O.

Over the past decade, pervasive research efforts have led to a renewed mechanistic understanding of NH₃-SCR over Cu-CHA, unveiling the atomic-scale structure of the main Cu-species involved.⁴⁻¹⁰ The reaction proceeds via Cu¹¹ to Cu¹ reduction, with release of the products. The catalytic cycle is then closed by reoxidation of Cu¹ to Cu¹¹, requiring the activation of O₂. The redox-active Cu ions in Cu-CHA are also known to dynamically respond to the gaseous feed across the relevant temperature window, switching between framework-coordinated and mobile configurations.²,¹¹

After heating a Cu-CHA catalyst at temperatures above 400 °C and in the presence of O₂, the Cu is present as a Cu¹¹ species, docked to the lattice oxygen atoms in correspondence of the Al exchange sites (Z) in the six- and eight-membered rings (6r and 8r) of the CHA zeolite. Assuming a random Al distribution in the zeolite framework, the chemical identity and local structure are determined by the catalyst composition: low Si/Al and Cu/Al ratios favor bare Z₂Cu¹¹ species in 6r, while at higher Si/Al and Cu/Al ratios an extra-ligand is required for charge compensation, resulting in Z[Cu¹¹OH] or oxygen-bridged multimeric Zₓ[Cuₓ¹¹Oᵧ] species preferentially hosted in 8r.¹²⁻¹⁴ It is worthwhile to note that deviations from the

random Al distribution, known to be promoted by specific synthesis approaches,¹⁵ could additionally influence the Cu-speciation in dehydrated Cu-CHA. Nonetheless, previous studies¹³,¹⁴,¹⁶ of the catalysts investigated herein point to a substantial agreement of Cu-speciation in the dehydrated state with the theoretical compositional phase diagram by Paolucci et al.,¹² based on a random Al distribution in the zeolite framework subject to the Löwenstein's rule.¹⁷

At 200 °C, the NH₃-SCR reaction proceeds in a quasi-homogeneous fashion, over NH₃-mobilized Cu-ions, yet electrostatically tethered to their framework exchange sites.⁶,¹⁸ Spectroscopic studies have been often performed by decoupling the reaction in the reduction and oxidation half-cycles, to facilitate the results interpretation. In the reduction half cycle exposure to a NO/NH₃ mixture, results in the reduction of all Cu ions to form [Cu¹(NH₃)₂]⁺ complexes. In the oxidation half-cycle, these [Cu¹(NH₃)₂]⁺ complexes are exposed to O₂, and the interaction of an O₂ molecule with a pair of [Cu¹(NH₃)₂]⁺ leads to the formation of [Cu₂(NH₃)₄O₂]²⁺ complexes, which can be described as a μ-η²,η²-peroxo diamino dicopper(II).¹⁹⁻²¹

Received: April 15, 2022

Accepted: June 21, 2022

Published: June 28, 2022

<figure><img src="image_7.png" /></figure>
<figure><img src="image_8.png" /><figcaption>**Figure 1.** *In situ* Cu K-edge XANES for (a) 0.1\_5, (b) 0.5\_15, and (c) 0.6\_29 Cu-CHA catalysts collected at 200 °C after pretreatment in O₂, at the end of the reduction step, during and after the oxidation step. Pie charts illustrate Cu¹/CuII percentages evaluated by XANES LCF at the end of the oxidation step for each catalyst; under the adopted experimental conditions, Cu¹ and CuII correspond to [Cu¹(NH₃)₂]⁺ and [Cu₂(NH₃)₄O₂]²⁺ complexes, respectively. (d–f) Pictorial representation of the main Cu-species expected at each step as a function of the catalyst composition, with open questions on parameters influencing coordination motif in [Cu₂(NH₃)₄O₂]²⁺ complexes in part (f).</figcaption></figure>

Paolucci et al. identified the volumetric Cu density as the key descriptor for the efficiency of the oxidation half cycle, validating that O₂ activation requires a [Cu¹(NH₃)₂]⁺ pair, leading to a quadratic dependency of the NH₃-SCR rate on Cu density at low Cu-loadings.⁶ Because the mobility of a

[Cu¹(NH₃)₂]⁺ complex is limited to distances below approximately 9 Å from their anchoring point in the zeolite, a low Cu density implies a lower propensity for [Cu¹(NH₃)₂]⁺ pair formation, and a larger fraction of unreacted [Cu¹(NH₃)₂]⁺. As the O₂ activation implies a change in the
<figure><img src="image_9.png" /><figcaption>**Figure 2.** (a) NOₓ conversion in the 150–500 °C temperature range for 0.1_5, 0.5_15, and 0.6_29. Amount of catalyst: 5 mg; feed gas: 500 ppm of NO, 533 ppm of NH₃, 5% H₂O, 10% O₂ in N₂; flow: 225 mL/min. The bottom inset correlates residual Cu¹ fractions evaluated by XANES LCF and turnover frequency (TOF) in mol/[mol<sub>Cu</sub> s] at 200 °C for the three catalysts. (b) Correlation between the same residual Cu¹ fractions and the volumetric Cu density in Cu-CHA catalysts, comparing experimental values obtained in this work (colored full circles) and literature values by Paolucci et al.⁶ (empty gray squares).</figcaption></figure>

oxidation state of Cu¹ to CuII, the fraction of unreacted [Cu¹(NH₃)₂]⁺ can be readily quantifiable by Cu K-edge X-ray Absorption Spectroscopy (XAS).

In this scenario, the actual reaction takes place on mobile Cu species, and therefore, the stable position of framework-bound Cu ions seems less relevant for the NH₃-SCR activity. However, the density and distribution of the framework Al atoms and Brønsted acid sites may influence the mobility of the [Cu¹(NH₃)₂]⁺ complexes, the stability of Cu pairs, and thus the formation of the [Cu₂(NH₃)₄O₂]²⁺ complexes. The potential implications for low-temperature NH₃-SCR performance through such zeolite-host driven changes in [Cu₂(NH₃)₄O₂]²⁺ formation are still unexplored.

To determine the influence of the zeolite properties on the NH₃-SCR reaction, we performed an *in situ* XAS study empowered by wavelet transform (WT) analysis and machine learning (ML)-assisted fitting of the extended X-ray absorption fine structure (EXAFS) spectra in order to interrogate three Cu-CHA catalysts with variable Si/Al ratios and Cu contents during the reduction and oxidation half-cycles in NH₃-SCR at 200 °C. Cu content and Si/Al ratio in the catalysts are balanced in such a way that the Cu density in two of the three catalysts is equivalent, despite having different Si/Al ratios. The catalysts used in this study have a Si/Al ratio of 5, 15 and 29, with a Cu/Al ratio of 0.1, 0.5, and 0.6 (estimated Cu densities of 0.28, 0.44, and 0.28 Cu/A³, respectively), denoted hereafter as “0.1_5”, “0.5_15”, and “0.6_29”. These catalysts have been characterized previously in depth after pretreatment in O₂ at 400 °C.¹⁴ We use the 0.5_15 catalyst as a reference, because it was previously investigated under the same redox conditions.²⁰ Additional details on the investigated catalysts, as well as on the experimental methods for *in situ* XAS data collection can be found in the SI, Section 1.

**Figure 1a–c** compares the Cu K-edge X-ray absorption near edge structure (XANES) spectra of the three catalysts measured after pretreatment in O₂ at 400 °C and cooling down to 200 °C in the same gas feed, at the end of the reduction step in NO/NH₃ and during the exposure of the reduced catalyst to O₂, also collected under isothermal conditions at 200 °C. In parallel, **Figure 1d–f** illustrates the main envisaged Cu-species at each step in this process.

For all three catalysts, the XANES after pretreatment in O₂ at 400 °C (dashed gray curves in **Figure 1**) shows the expected features for Z₂CuII and Z[CuIIOH]/Zₓ[CuₓIIOᵧ] species, reflecting their different Cu/Al and Si/Al ratios.¹²⁻¹⁴ At the end of the reduction step, for each catalyst, the XANES indicates the formation of mobile [Cu¹(NH₃)₂]⁺ for all the Cu ions present. For the 0.1_5 composition, the reduction to [Cu¹(NH₃)₂]⁺ of the dominant Z₂CuII species implies the formation of a new Brønsted acid site to maintain the charge balance in the zeolite. As NH₃ is present in the applied reduction conditions, this results in the formation of NH₄⁺ ions (**Figure 1e**).

During the oxidation step, the characteristic XANES features of CuII progressively develop, in line with the formation of [Cu₂(NH₃)₄O₂]²⁺ complexes.⁶,²⁰ However, the spectral shape reached at the end of the oxidation step for the 0.1_5 catalyst differs from those observed for the 0.5_15 and 0.6_29 catalysts, especially in the white-line peak region. This indicates a different coordination motif for [Cu₂(NH₃)₄O₂]²⁺ in the Al-rich 0.1_5 catalyst, and therefore, we undertook a more in-depth analysis of the *in situ* XAS data.

Although the majority of the Cu ions are reoxidized to CuII after the oxidation step, from XANES linear combination fit (LCF) we found a residual amount of [Cu¹(NH₃)₂]⁺, determined by CHA Si/Al ratio, and ranging from 13% for Si/Al = 5, to 16% for Si/Al = 15 and 24% for Si/Al = 29 (see pie charts in **Figure 1a–c** and SI, Section 2 for details).

**Figure 2a** reports the NOₓ conversion in NH₃-SCR for the three catalysts as a function of temperature. At 200 °C, 0.1_5 and 0.5_15 show almost equivalent conversion, which is instead lower for 0.6_29. The inset of **Figure 2a** correlates the turnover frequency (TOF), obtained by converting the measured NOₓ conversion at 200 °C to a rate constant based on a first order kinetic model, corresponding to an integral reactor analysis,²² and accounting for Cu wt % in the catalysts (SI, Table S1). Considering the increase in residual Cu¹ as Si/Al increases observed from XANES LCF, the TOF at 200 °C follows the opposite trend: it is higher in 0.1_5 and it decreases in an approximately linear way for the 0.5_15 and 0.6_29 catalysts. This indicates that a more efficient oxidation of [Cu¹(NH₃)₂]⁺ by O₂ activation is beneficial for the low-temperature NH₃-SCR performance.
<figure><img src="image_10.png" /><figcaption>**Figure 3.** Snapshots of local coordination environment of Cu ions by EXAFS, comparing 0.1\_5, 0.5\_15 and 0.6\_29 at the end of the (a, b) reduction and (c, d) oxidation steps. (a, c) Magnitude of FT-EXAFS spectra, obtained by Fourier transforming $k^2\chi(k)$ spectra in the 2.4–12.0 Å⁻¹ range. (b, d) Corresponding EXAFS-WT maps, magnified in the 2–4 Å range and plotted using a common intensity scale. Low-R (LR) and high-R (HR) features in the *k*-range diagnostic of Cu–Cu scattering are highlighted by white arrows in part (d).</figcaption></figure>

<figure><img src="image_11.png" /><figcaption>**Figure 4.** (a) Molecular models for the structural components included in the Machine Learning (ML)-assisted EXAFS fitting model: 1 [Cu¹(NH₃)₂]⁺, 2 "planar", and 3 "bent" motifs for µ-η²,η²-peroxo diamino dicopper(II); when relevant, characteristic EXAFS-derived ranges for Cu–Cu interatomic distances are reported, in Å. (b–d) Comparison between magnitudes of experimental (colored circles) and best fit (thick lines) FT-EXAFS spectra at the end of the oxidation step for (b) 0.1\_5, (c) 0.5\_15, and (d) 0.6\_29 (see SI, Figure S13 for the corresponding imaginary parts). The scaled components for Cu-species 1, 2/2', 3 are also reported, vertically translated for the sake of clarity, together with percentages of each component over total Cu refined by ML-EXAFS fitting.</figcaption></figure>

We note that the difference in residual Cu¹ fractions is not entirely determined by the Cu density, but that the Si/Al ratio also plays a role. Figure 2b compares Cu density with the residual Cu¹ fraction for the three catalysts investigated in this study and for the data by Paolucci et al.⁶ It is worth noticing that the 0.1\_5 and 0.6\_29 catalysts show comparable Cu density, while the residual Cu¹ fraction after oxidation is significantly lower for 0.1\_5 than for 0.6\_29. The data appear to branch based on the Si/Al ratio, with a different dependence on the Cu density for low and high Si/Al ratios (purple and blue shadowed areas in Figure 2b, for Si/Al = 5 and Si/Al = 15, 29, respectively). Overall, at comparable Cu density, for Si/Al = 5 a lower residual Cu¹ fraction is observed than for higher Si/

Al ratios. This behavior is reminiscent of the compositional effects on Cu-speciation after pretreatment in O₂, when low Si/Al favors Z₂Cu¹¹ at the expense of Z[Cu¹¹OH]¹²,¹³ although the oxidation step proceeds from mobile [Cu¹(NH₃)₂]⁺, spectroscopically indistinguishable over the compositional series.

To correlate quantitatively the structural differences in the CHA zeolites with the observed trends in oxidation efficiency, we compared the EXAFS of the three catalysts at the end of both the reduction and oxidation steps (Figure 3). Together with the conventional Fourier transform (FT)-EXAFS representation, we exploited a WT-based analysis²,²⁴ to unambiguously identify possible Cu–Cu scattering contribu-
tions possessing a characteristic lobe centered at ca. 7 Å⁻¹ along the *k* direction¹⁴,²⁰,²⁵⁻²⁸ (SI, Section 3 for details).

EXAFS confirms that after the reduction step all the Cu is present as [Cu¹(NH₃)₂]⁺ complexes, without any detectable dependence on the Cu and Al contents in the catalyst (Figure 3a,b). In all cases, unstructured FT-EXAFS features are observed beyond the first-shell peak originating from Cu–N single scattering. In parallel, the WT maps only shows a low-k lobe assigned to multiple scattering paths involving the two N atoms of the NH₃ ligands. EXAFS fits based on the [Cu¹(NH₃)₂]⁺ structure confirmed this picture (SI, Section 4.2).

In all cases, the FT-EXAFS shows a first-shell peak with the same intensity at the end of the oxidation step, indicating 4-fold coordinated Cu¹I ions. In the R-range within 2–4 Å, a broad peak centered at 2.5 Å grows in intensity in the order 0.1–5 < 0.5–15 < 0.6–29, accompanied by further variations in the 3–4 Å range (Figure 3c). The WT maps show a low-k lobe originating from multiple scattering contributions from low-Z (O and N) neighbors for all catalysts (see Figure 3d and SI, Figure S5b for the corresponding ΦR(k) density power functions), with an intensity and R-space location that is only slightly affected by the catalyst composition. In the high-k range characteristic of Cu–Cu scattering, we observe two local maxima along the *R* direction at ca. 2.5 and 3.2 Å (LR and HR labels in Figure 3d, respectively), pointing to an EXAFS-resolvable bimodal distribution of Cu–Cu interatomic distances. The LR feature becomes more intense relative to the HR feature as the Si/Al ratio increases; the HR feature is also inherently weaker due to the dampening of the EXAFS signal as *R* increases.

Taking into account phase correction, the **HR** feature is compatible with the DFT-optimized geometry of quasi-planar µ-η²,η²-peroxo diamino dicopper(II) with intranuclear separation of 3.40 Å, as reported for 0.5–15 in our previous work.²⁰ However, the conventional EXAFS refinement solely based on this model revealed a local lack of fit at ca. 2.5 Å (SI, Section 4.3). This corresponds to the **LR** feature becoming more visible for 0.6–29 in the WT maps.

To further understand the emerging structural complexity, we employed a novel ML-assisted EXAFS analysis approach²⁹⁻³¹ to build up a robust three-component fitting model. The model accounts for a minor presence of [Cu¹(NH₃)₂]⁺ (Figure 4a, 1) and for a bimodal distribution of the Cu–Cu distances in µ-η²,η²-peroxo diamino dicopper(II). On the basis of the WT analysis, the latter is described by combining contributions from the already proposed quasi-planar configuration (Figure 4a, 2/2') and a “bent” motif (Figure 4a, 3) for the same complex, refined through ML-based optimization of the Cu–O–Cu angle (see SI, Section 5 for a detailed description of the methodology and a complete report on fitting results).

Figure 4b–d compares the corresponding experimental and best-fit EXAFS spectra for the three catalysts, highlighting the individual scattering contributions and refined percentage for each Cu-species. The percentages of residual [Cu¹(NH₃)₂]⁺ agree well with those from XANES LCF, revealing the same trend in the oxidation efficiency as a function of the Si/Al ratio. The previously observed lack of fit at ca. 2.5 Å is now resolved for the whole set of samples.

The fit confirms that two distinct µ-η²,η²-peroxo diamino dicopper(II) coordination motifs are required to fully model the EXAFS of 0.5–15 and 0.6–29, which is reflected in a

different Cu–Cu distance for the bent (3.03–3.06 Å) and planar complex (3.34–3.39 Å). Interestingly, for 0.1–5 the three-component fit restitutes Cu–Cu distances of 3.38 and 3.39 Å, not distinguishable within the accuracy of EXAFS analysis and both pointing to the same planar motif (2/2' labels in Figure 4b). The bent motif is instead progressively favored as the Si/Al ratio increases, becoming the major structural component for the 0.6–29 sample.

ML-EXAFS fitting ensures a quantitative understanding of the subtle differences observed in the XANES spectral shape as well as in the high-R portion of WT maps, where the LR/HR features fairly match the optimized Cu–Cu distances for planar and bent µ-η²,η²-peroxo diamino dicopper(II). The adopted approach allows refining, in principle, any structure starting from an initially guessed molecular complex with significantly different interatomic distances and angles. These results therefore highlight the potential of *in situ* XAS combined with integrated WT and ML-assisted EXAFS analysis.

Summarizing, the XANES and EXAFS results for the Cu-CHA catalysts consistently show, that the Si/Al ratio of the zeolite host affects the structure of mobile dicopper(II) complexes formed during the oxidation of the [Cu¹(NH₃)₂]⁺ complexes by O₂. Diffuse Reflectance UV–vis spectroscopy, qualitatively responsive to the structure of Cu-oxo species, further supports these results (see SI, Section 6). Therefore, we suggest that the diverse electrostatic landscape and the higher Brønsted acid site density in Al-rich zeolites could trigger host–guest interactions promoting a longer internuclear separation in the planar µ-η²,η²-peroxo diamino dicopper(II) motif. Plausibly, the NH₃ ligands in the dicopper(II) complex could participate into H-bonding interactions with ZH sites, as well as ZNH₄ and ZNH₄ nNH₃ associations, most likely formed at the reduction step in the presence of NH₃ at 200 °C,³² triggering the observed elongation effect in Cu–Cu distances. Importantly, this is accompanied by a more efficient oxidation at a given volumetric Cu density, which is beneficial for the NOₓ conversion under NH₃-SCR conditions at 200 °C. With this respect, Al-rich zeolites could favor dynamic Cu ion exchange between nearby sites, thus enhancing the mobility of [Cu¹(NH₃)₂]⁺ complexes beyond the limit dictated by electrostatic tethering to the initial exchange sites. A similar mechanism based on H⁺/H₂O-aided diffusion of Cu¹ was proposed in the context of continuous partial oxidation of methane to methanol over Cu-CHA, although in this case ZNH₄ is suggested to hinder the exchange pathway.³³ Overall, the findings obtained in this work provide a robust experimental basis for further theoretical modeling of low-temperature NH₃-SCR mechanism, aimed at validating these hypotheses within a quasi-homogeneous Cu-catalyzed oxidation half-cycle actively driven by the compositional characteristics of the zeolitic host.

<figure><img src="image_12.png" /></figure>

## ASSOCIATED CONTENT

<figure><img src="image_13.png" /></figure>

### Supporting Information

The Supporting Information is available free of charge at
https://pubs.acs.org/doi/10.1021/acs.jpclett.2c01107.

Details on compositional characteristics, evaluation of Cu density and synthesis methods for the investigated Cu-CHA catalysts. Experimental methods for *in situ* XAS and UV–vis spectroscopies. Additional information about methods, models and supplementary results for the employed XAS data analysis strategies: XANES LCF,
EXAFS WT, conventional EXAFS fitting, and ML-assisted EXAFS fitting. Complementary *in situ* UV–vis spectroscopy results (PDF)

■ AUTHOR INFORMATION

**Corresponding Author**

Elisa Borfecchia - Department of Chemistry and NIS Centre,
University of Turin, 10125 Turin, Italy; orcid.org/0000-0001-8374-8329; Email: elisa.borfecchia@unito.it

**Authors**

Andrea Martini - Department of Chemistry and NIS Centre,
University of Turin, 10125 Turin, Italy; Present
Address: A.M.: Interface Science Department, Fritz Haber
Institute, Faradayweg 4-6, 14195 Berlin, Germany

Chiara Negri - Department of Chemistry and NIS Centre,
University of Turin, 10125 Turin, Italy; Present
Address: C.N.: Politecnico di Milano, Laboratory of
Catalysis and Catalytic Processes, Department of Energy,
via La Masa, 34, 20156 Milano, Italy

Luca Bugarin - Department of Chemistry and NIS Centre,
University of Turin, 10125 Turin, Italy; European
Synchrotron Radiation Facility, 38043 Grenoble Cedex 9,
France

Gabriele Deplano - Department of Chemistry and NIS
Centre, University of Turin, 10125 Turin, Italy

Reza K. Abasabadi - Department of Chemistry and NIS
Centre, University of Turin, 10125 Turin, Italy

Kirill A. Lomachenko - European Synchrotron Radiation
Facility, 38043 Grenoble Cedex 9, France

Ton V. W. Janssens - Umicore Denmark ApS, DK-2970
Hørsholm, Denmark

Silvia Bordiga - Department of Chemistry and NIS Centre,
University of Turin, 10125 Turin, Italy; orcid.org/0000-0003-2371-4156

Gloria Berlier - Department of Chemistry and NIS Centre,
University of Turin, 10125 Turin, Italy; orcid.org/0000-0001-7720-3584

Complete contact information is available at:
https://pubs.acs.org/10.1021/acs.jpclett.2c01107

**Notes**

The authors declare no competing financial interest.

■ ACKNOWLEDGMENTS

The authors acknowledge funding from project n. 2017KKPSZ PRIN-2017 MOSCATo (Cutting-edge X-ray methods and models for the understanding of surface site reactivity in heterogeneous catalysts and sensors); Horizon 2020 Excellence Science ERC-Synergy program 2019-CUBE: “Unravelling the secrets of Cu-based catalysts for C–H activation” (grant agreement no. 856446); European Union’s Horizon 2020 research and innovation programme under the Marie Skłodowska-Curie grant agreement no. 955839 (CHASS). This work reflects only the authors’ view, and the Agency is not responsible for any use that can be made of the information it contains. The European Synchrotron Radiation Facility (ESRF, Grenoble, France) is acknowledged for beamtime allocation on the BM23 beamline. The authors are grateful to T. Selleri for help during the XAS experiments, as well as to P. N. Vennestrøm and A. Molokova for insightful discussions.

■ REFERENCES

(1) Beale, A. M.; Gao, F.; Lezcano-Gonzalez, I.; Peden, C. H. F.; Szanyi, J. Recent Advances in Automotive Catalysis for NOₓ Emission Control by Small-Pore Microporous Materials. *Chem. Soc. Rev.* **2015**, *44*, 7371–7405.

(2) Borfecchia, E.; Beato, P.; Svelle, S.; Olsbye, U.; Lamberti, C.; Bordiga, S. Cu-CHA - A Model System for Applied Selective Redox Catalysis. *Chem. Soc. Rev.* **2018**, *47*, 8097–8133.

(3) Gao, F.; Peden, C. H. F. Recent Progress in Atomic-Level Understanding of Cu/SSZ-13 Selective Catalytic Reduction of Redox Catalysts. *Catalysts* **2018**, *8*, 140.

(4) Janssens, T. V. W.; Falsig, H.; Lundegaard, L. F.; Vennestrøm, P. N. R.; Rasmussen, S. B.; Moses, P. G.; Giordanino, F.; Borfecchia, E.; Lomachenko, K. A.; Lamberti, C.; Bordiga, S.; Godiksen, A.; Mossin, S.; Beato, P. A Consistent Reaction Scheme for the Selective Catalytic Reduction of Nitrogen Oxides with Ammonia. *ACS Catal.* **2015**, *5*, 2832–2845.

(5) Lomachenko, K. A.; Borfecchia, E.; Negri, C.; Berlier, G.; Lamberti, C.; Beato, P.; Falsig, H.; Bordiga, S. The Cu-CHA deNOₓ Catalyst in Action: Temperature-Dependent NH₃-Assisted Selective Catalytic Reduction Monitored by Operando XAS and XES. *J. Am. Chem. Soc.* **2016**, *138*, 12025–12028.

(6) Paolucci, C.; Khurana, I.; Parekh, A. A.; Li, S. C.; Shih, A. J.; Li, H.; Di Iorio, J. R.; Albarracin-Caballero, J. D.; Yezerets, A.; Miller, J. T.; Delgass, W. N.; Ribeiro, F. H.; Schneider, W. F.; Gounder, R. Dynamic Multinuclear Sites Formed by Mobilized Copper Ions in NOₓ Selective Catalytic Reduction. *Science* **2017**, *357*, 898–903.

(7) Marberger, A.; Petrov, A. W.; Steiger, P.; Elsener, M.; Krocher, O.; Nachtegaal, M.; Ferri, D. Time-Resolved Copper Speciation During Selective Catalytic Reduction of NO on Cu-SSZ-13. *Nat. Catal.* **2018**, *1*, 221–227.

(8) Chen, L.; Janssens, T. V. W.; Vennestrøm, P. N. R.; Jansson, J.; Skoglundh, M.; Grönbeck, H. A Complete Multisite Reaction Mechanism for Low-Temperature NH₃-SCR over Cu-CHA. *ACS Catal.* **2020**, *10*, 5646–5656.

(9) Hu, W.; Selleri, T.; Gramigni, F.; Fenes, E.; Rout, K. R.; Liu, S.; Nova, I.; Chen, D.; Gao, X.; Tronconi, E. On the Redox Mechanism of Low-Temperature NH₃-SCR over Cu-CHA: A Combined Experimental and Theoretical Study of the Reduction Half Cycle. *Angew. Chem., Int. Ed.* **2021**, *60*, 7197–7204.

(10) Feng, Y.; Wang, X.; Janssens, T. V. W.; Vennestrøm, P. N. R.; Jansson, J.; Skoglundh, M.; Grönbeck, H. First-Principles Microkinetic Model for Low-Temperature NH₃-Assisted Selective Catalytic Reduction of NO over Cu-CHA. *ACS Catal.* **2021**, *11*, 14395–14407.

(11) Krishna, S. H.; Jones, C. B.; Miller, J. T.; Ribeiro, F. H.; Gounder, R. Combining Kinetics and Operando Spectroscopy to Interrogate the Mechanism and Active Site Requirements of NOₓ Selective Catalytic Reduction with NH₃ on Cu-Zeolites. *J. Phys. Chem. Lett.* **2020**, *11*, 5029–5036.

(12) Paolucci, C.; Parekh, A. A.; Khurana, I.; Di Iorio, J. R.; Li, H.; Albarracin Caballero, J. D.; Shih, A. J.; Anggara, T.; Delgass, W. N.; Miller, J. T.; Ribeiro, F. H.; Gounder, R.; Schneider, W. F. Catalysis in a Cage: Condition-Dependent Speciation and Dynamics of Exchanged Cu Cations in SSZ-13 Zeolites. *J. Am. Chem. Soc.* **2016**, *138*, 6028–6048.

(13) Martini, A.; Borfecchia, E.; Lomachenko, K. A.; Pankin, I. A.; Negri, C.; Berlier, G.; Beato, P.; Falsig, H.; Bordiga, S.; Lamberti, C. Composition-Driven Cu-Speciation and Reducibility in Cu-CHA Zeolite Catalysts: A Multivariate XAS/FTIR Approach to Complexity. *Chem. Sci.* **2017**, *8*, 6836–6851.

(14) Negri, C.; Martini, A.; Deplano, G.; Lomachenko, K. A.; Janssens, T. V. W.; Borfecchia, E.; Berlier, G.; Bordiga, S. Investigating the Role of Cu-Oxo Species in Cu-Nitrate Formation over Cu-CHA Catalysts. *Phys. Chem. Chem. Phys.* **2021**, *23*, 18322–18337.

(15) Di Iorio, J. R.; Gounder, R. Controlling the Isolation and Pairing of Aluminum in Chabazite Zeolites Using Mixtures of Organic and Inorganic Structure-Directing Agents. *Chem. Mater.* **2016**, *28*, 2236–2247.
(16) Pappas, D. K.; Borfecchia, E.; Dyballa, M.; Pankin, I. A.; Lomachenko, K. A.; Martini, A.; Signorile, M.; Teketel, S.; Arstad, B.; Berlier, G.; Lamberti, C.; Bordiga, S.; Olsbye, U.; Lillerud, K. P.; Svelle, S.; Beato, P. Methane to Methanol: Structure Activity Relationships for Cu-CHA. *J. Am. Chem. Soc.* **2017**, *139*, 14961–14975.

(17) Löwenstein, W. The Distribution of Aluminum in the Tetrahedra of Silicates and Aluminates. *Am. Mineral.* **1954**, *39*, 92–96.

(18) Gao, F.; Mei, D.; Wang, Y.; Szanyi, J.; Peden, C. H. F. Selective Catalytic Reduction over Cu/SSZ-13: Linking Homo- and Heterogeneous Catalysis. *J. Am. Chem. Soc.* **2017**, *139*, 4935–4942.

(19) Chen, L.; Falsig, H.; Janssens, T. V. W.; Grönbeck, H. Activation of Oxygen on (NH₃CuNH₃)⁺ in NH₃-SCR over Cu-CHA. *J. Catal.* **2018**, *358*, 179–186.

(20) Negri, C.; Selleri, T.; Borfecchia, E.; Martini, A.; Lomachenko, K. A.; Janssens, T. V. W.; Cutini, M.; Bordiga, S.; Berlier, G. Structure and Reactivity of Oxygen-Bridged Diamino Dicopper(II) Complexes in Cu-Ion-Exchanged Chabazite Catalyst for NH₃-Mediated Selective Catalytic Reduction. *J. Am. Chem. Soc.* **2020**, *142*, 15884–15896.

(21) Oda, A.; Shionoya, H.; Hotta, Y.; Takewaki, T.; Sawabe, K.; Satsuma, A. Spectroscopic Evidence of Efficient Generation of Dicopper Intermediate in Selective Catalytic Reduction of NO over Cu-Ion-Exchanged Zeolites. ACS Catal. **2020**, *10*, 12333–12339.

(22) Levenspiel, O. *Chemical Reaction Engineering*, 3rd ed.; Wiley: New York, 1999.

(23) Funke, H.; Scheinost, A. C.; Chukalina, M. Wavelet Analysis of Extended X-Ray Absorption Fine Structure Data. *Phys. Rev. B* **2005**, *71*, 094110.

(24) Timoshenko, J.; Kuzmin, A. Wavelet Data Analysis of EXAFS Spectra. *Comput. Phys. Commun.* **2009**, *180*, 920–925.

(25) Pankin, I. A.; Martini, A.; Lomachenko, K. A.; Soldatov, A. V.; Bordiga, S.; Borfecchia, E. Identifying Cu-Oxo Species in Cu-Zeolites by XAS: A Theoretical Survey by DFT-Assisted XANES Simulation and EXAFS Wavelet Transform. *Catal. Today* **2020**, *345*, 125–135.

(26) Sushkevich, V. L.; Safonova, O. V.; Palagin, D.; Newton, M. A.; van Bokhoven, J. A. Structure of Copper Sites in Zeolites Examined by Fourier and Wavelet Transform Analysis of EXAFS. *Chem. Sci.* **2020**, *11*, 5299–5312.

(27) Martini, A.; Signorile, M.; Negri, C.; Kvande, K.; Lomachenko, K. A.; Svelle, S.; Beato, P.; Berlier, G.; Borfecchia, E.; Bordiga, S. EXAFS Wavelet Transform Analysis of Cu-MOR Zeolites for the Direct Methane to Methanol Conversion. *Phys. Chem. Chem. Phys.* **2020**, *22*, 18950–18963.

(28) Deplano, G.; Martini, A.; Signorile, M.; Borfecchia, E.; Crocellà, V.; Svelle, S.; Bordiga, S. Copper Pairing in the Mordenite Framework as a Function of the Cu¹/Cu¹¹ Speciation. *Angew. Chem., Int. Ed.* **2021**, *60*, 25891–25896.

(29) Martini, A.; Guda, S. A.; Guda, A. A.; Smolentsev, G.; Algasov, A.; Usoltsev, O.; Soldatov, M. A.; Bugaev, A.; Rusalev, Y.; Lamberti, C.; Soldatov, A. V. PyFitit: The Software for Quantitative Analysis of XANES Spectra Using Machine-Learning Algorithms. *Comput. Phys. Commun.* **2020**, *250*, 107064.

(30) Martini, A.; Bugaev, A. L.; Guda, S. A.; Guda, A. A.; Priola, E.; Borfecchia, E.; Smolders, S.; Janssens, K.; De Vos, D.; Soldatov, A. V. Revisiting the Extended X-ray Absorption Fine Structure Fitting Procedure through a Machine Learning-Based Approach. *J. Phys. Chem. A* **2021**, *125*, 7080–7091.

(31) Guda, A. A.; Guda, S. A.; Martini, A.; Kravtsova, A. N.; Algasov, A.; Bugaev, A.; Kubrin, S. P.; Guda, L. V.; Šot, P.; van Bokhoven, J. A.; Copéret, C.; Soldatov, A. V. Understanding X-Ray Absorption Spectra by Means of Descriptors and Machine Learning Algorithms. *NPJ. Comput. Mater.* **2021**, *7*, 203.

(32) Giordanino, F.; Borfecchia, E.; Lomachenko, K. A.; Lazzarini, A.; Agostini, G.; Gallo, E.; Soldatov, A. V.; Beato, P.; Bordiga, S.; Lamberti, C. Interaction of NH₃ with Cu-SSZ-13 Catalyst: A Complementary FTIR, XANES, and XES Study. *J. Phys. Chem. Lett.* **2014**, *5*, 1552–1559.

(33) Dinh, K. T.; Sullivan, M. M.; Narsimhan, K.; Serna, P.; Meyer, R. J.; Dincă, M.; Román-Leshkov, Y. Continuous Partial Oxidation of Methane to Methanol Catalyzed by Diffusion-Paired Copper Dimers in Copper-Exchanged Zeolites. *J. Am. Chem. Soc.* **2019**, *141*, 11641–11650.

<figure><img src="image_14.png" /></figure>

Recommended for ACS

Hydrothermal Aging Alleviates the Phosphorus Poisoning of Cu-SSZ-39 Catalysts for NH₃-SCR Reaction

Junlin Chen, Hong He, et al.

FEBRUARY 22, 2023

ENVIRONMENTAL SCIENCE & TECHNOLOGY

<figure><img src="image_15.png" /></figure>

<figure><img src="image_16.png" /></figure>

Influence of Solvent on Selective Catalytic Reduction of Nitrogen Oxides with Ammonia over Cu-CHA Zeolite

Jamal Abdul Nasir, Alexey A. Sokol, et al.

DECEMBER 22, 2022

JOURNAL OF THE AMERICAN CHEMICAL SOCIETY

<figure><img src="image_17.png" /></figure>

<figure><img src="image_18.png" /></figure>

Highlights on Key Roles of Y on the Hydrothermal Stability at 900 °C of Cu/SSZ-39 for NH₃-SCR

Qingjin Lin, Yaoqiang Chen, et al.

OCTOBER 31, 2022

ACS CATALYSIS

<figure><img src="image_19.png" /></figure>

<figure><img src="image_20.png" /></figure>

Realizing and Revealing Complex Isobutyl Alcohol Production over a Simple Cu-ZrO₂ Catalyst

Nana Gong, Yisheng Tan, et al.

FEBRUARY 27, 2023

ACS CATALYSIS

<figure><img src="image_21.png" /></figure>

<figure><img src="image_22.png" /></figure>

Get More Suggestions >